Filament Feed Materials for Fused Deposition Processing of ... Filament Feed Materials for Fused...
Embed Size (px)
Transcript of Filament Feed Materials for Fused Deposition Processing of ... Filament Feed Materials for Fused...
Filament Feed Materials for Fused Deposition Processing of Ceramics and Metals
M.K. Agarwala, R. van Weeren, A. Bandyopadhyay, A. Safari, and S.C. Danforth
Center for Ceramic Research, Rutgers University
W.R. Priedeman Stratasys Inc.
Fused Deposition of Ceramics (FDC) and Metals (FDMet) are SFF techniques, based on commercial FDMTM technology, for fabrication of ceramic and metal components. The FD processes use feed material in the form of filaments which require certain phy~ical and mechanical properties. FDC and FDMet processes employ fila.n::ents formed from ?erannc ~r metal powders mixed with thermoplastic polymers. The thermoplastic polymers act as bmder dunng the FDC and FDMet processing in forming a green part. Development of green ceramic or metal fIlaments for FDC or FDMet processing involves three critical steps : selection of an appropriate binder chemistry, appropriate mixing procedures and fIlament fabrication techniques. This study describes the properties required for filaments for successful FD processing and the approach taken in the development of a series of binder which meets these requisite properties for a wide range of ceramics and metals. Appropriate mixing and filament forming techniques are also discussed.
Most of the SFF techniques for fabrication of ceramic and metal parts employ polymeric binder systems to bond the ceramic or metal particles together in forming a green part . The green part is then processed to remove the binder from the part and then sintered or infIltrated with a lower melting second phase . However, fabrication of green ceramic or metal parts by various SFF techniques have been far from trivial. First, effort is required in developing the proper binder chemistry to allow SFF processing. In addition, effort may be needed in developing suitable dispersants for the specific particulate system and the binder chemistry. Once an appropriate binder chemistry and dispersant have been selected, the ceramic or metal powder systems are processed with the binder and dispersant to form the feedstock in a suitable physical form (powder, sheets, filaments) for specific SFF processing .
Each SFF technique requires feedstock materials with certain physical and mechanical properties. .Poor selection of binder chemistry, dispersant, and poor processing of the feedstock can lead to unsuccessful SFF processing. This study describes the development of green ceramic and metal fIlament feedstocks for successful processing by Fused Deposition of Ceramics (FDC) and Metals (FDMet). FDC and FDMet are SFF techniques, based on commercial FDMTM technology, which are being developed for a wide range of ceramics and metals to produce complex shaped ceramic and metal parts with functional properties [2-5]. This study discusses the various physical and mechanical properties required in the filament feedstock for successful FD processing. The study also describes the development of a binder system and the filament fabrication procedures employed for various ceramic and metal systems.
ll. Filament Feedstock Characteristics for FD Processing
The commercial FDMTM systems fabricate wax and polymer parts using continuous spooled fIlaments as the feed material. The filament is fed through a position-controlled heated liquefier head which deposits molten material in precise locations [6,7]. For the filament to be successfully fed into the liquefier and extruded in molten form out of a nozzle, the filament must have certain properties. The fIlament, which is fed into the liquefier head by a pair of counter- rotating rollers, not only acts as the feed material, but also serves as an efficient piston for extrusion. Therefore, for a certain material viscosity the filament must have sufficient stiffness and
strength for extrusion, or else the filament will buckle or break after passing through the rollers and not be successful in extruding material [5,7]. Hence, necessary, but not sufficient, conditions for successful FD processing are low viscosity and high stiffness. In addition, the material must have good adhesive behavior for bonding between adjacent roads and layers of deposited material [5,7].
Although filaments with low viscosity, high stiffness, and good adhesion characteristics are sufficient to establish FD processing feasibility, for complete process optimization and automation, the filament feedstock must also posses high flexural modulus and flexural strength [5,7]. High flexural modulus and strength are needed to enable continuous spooling of the filaments onto a spool to provide continuous feedstock supply for the FDMTM system. These properties are also necessary to allow continuous un-spooling of the filament from the spool for uninterrupted feeding (without breaking of the filaments) of the liquefier during fabrication.
FDC and FDMet processing, using commercial FDMTM systems, require development of powderlbinder filament feedstocks with the above mentioned properties, namely, low viscosity, high stiffness, good adhesion behavior, high flexural modulus and strength. This is done through binder development and selection of dispersant. In addition to these constraints, development of binder(s) and dispersant for FDC or FDMet must also address issues commonly relevant to all green forming techniques. The binder and dispersant have as high a solids loading as possible (>50 volume%), have good dispersion behavior, and must leave no residue after binder removal.
III. Binders for FDC and FDMet
The binders for green forming techniques typically consist of many components; each added for a specific role in the final mix. In this study a four component binder system has been developed for FDC and FDMet processing. As shown in Table I, each of these components plays a specific role in the final formulation. Table I also shows the temperature range at which each of these components volatilize during binder removal. The amount of each component in the formulation used for FDC or FDMet is varied to tailor the properties needed to allow successful FD processing of specific ceramic or metal system. The weight percent of each of these components varied in this study for FDC/FDMet is also shown in Table I. This binder system is designated RUx (x is the identification number of a particular binder formulation under consideration) .
The particulate systems studied for FDC and FDMet processing to date include silicon nitride, silica, lead zirconium titanate (PZT), stainless steel, and tungsten carbide-cobalt. Initial feasibility studies for each of these particulate systems were done by using the RU1 binder formulation which contains 30% wax, 35% polymer, 15% tackifier, and 20% elastomer by weight. 50 to 65 volume % powders were mixed the RU1 binder and fabricated into filaments for FD feasibility studies. In addition, viscosity measurements were made on the mixed feedstock. Based on the viscosity behavior and FD feasibility studies, the binder formulation were further optimized. Also, dispersants were selected and used for certain particulate systems to facilitate FD processing. Depending on the study done with each particulate system, the binder formulation development and dispersant selection was either limited to developing filaments which are FD process worthy but not flexible or was developed to produce FD process worthy and continuous and flexible filaments. Table IT shows the different RU binder formulations used successfully for FDC and FDMet processing of various materials. The Table also shows the amount of powder used for FD processing of each system and the nature of the filament feedstock thus produced.
Binder and Dispersant Development for FDC of Silicon Nitride
Most significant FD process development to date has been done with Si3N4 [3-5]. Although initial FDC trials of 60 volume % Si3N4 with RU1 binder formulation were successful, the filaments were rigid and not flexible enough to enable spooling for continuous and automated
FDC processing. To facilitate continuous and automated FDC processing of Si3N4, the RU binder was tailored and optimized by a linear Design of Experiments (DoE) . Nine different RU fonnulations with a wide range of wax. polymer, tackifier, and elastomer contents were used. Viscosity measurements were made on each of these compositions as a function of te:n~eratureand shear rate to get the viscosity response as a function of each of 0e co~ponen.ts. Slt~:nlarly, gI~ss transition temperatures (Tg) were measured for each fonnuiatlon uSIng D~ferentlal Scannmg Calorimetry. Tg is commonly used as an indicator of the flexi~ility of the matenal. The. d~?t from the DoE was analyzed to determine the effects of the vanous components on fleXIbility and viscosity. Using a linear representations of the response,
Response =Co + Cl [tackifier] + C2 [elastomer] + C3 [polymer] + C4 [wax]
the coefficients (Co -(4) for the effect of each component on viscosity and flexibility were calculated . From this linear DoE study, the following conclusions were drawn:
• The tackifier and elastomer improve flexibility and the wax adversely affects the flexibility. • Elastomer increases the viscosity and the wax lowers the viscosity.
Based on the results of DoE, the binder system RU9 was developed. RU9 formulation contains 20% wax, 19% polymer, 35% tackifier, and 26% elastomer by weight. In addition to developing RU9 binder formulation, a suitable dispersant was also selected. Selection of oleyl alcohol as dispersant was done by a screening process from among several commonly used dispersants for ceramics, especially silicon nitride . The screening of dispersants was done by measuring the viscosity of 30 volume % Si3N